The Influence of the Chelating Agent Nitrilotriacetic Acid on
A publication of
CHEMICAL ENGINEERING TRANSACTIONS
VOL. 32, 2013
The Italian Association
of Chemical Engineering
Online at: www.aidic.it/cet
Chief Editors: Sauro Pierucci, Jiří J. Klemeš
Copyright © 2013, AIDIC Servizi S.r.l.,
ISBN 978-88-95608-23-5; ISSN 1974-9791
The Influence of the Chelating Agent Nitrilotriacetic Acid on
Promotion of Hydrodesulfurization Activity by Co in CoMo
Catalysts Prepared on Al2O3, C, and ZrO2 Supports
Luděk Kaluža*, Miroslav Zdražil, Daniela Gulková, Zdeněk Vít
Institute of Chemical Process Fundamentals of the ASCR, v. v. i.; Rozvojová 135; 165 02 Prague 6 – Suchdol; Czech
Increasingly stringent regulations on sulfur level in liquid fuels have been recently driving the research on
highly active hydrodesulfurization (HDS) catalysts. The conventional CoMo catalysts are supported onto
gamma-Al2O3 and they are mostly prepared by consecutive deposition of ammonium heptamolybdate and
cobalt nitrate followed by calcination and sulfidation. Alternatively, chelating agent such as nitrilotriacetic
acid (NTA) is employed during the preparation to increase the HDS activity. In the present paper, a new
method based on impregnation of unconventional supports (i.e. activated carbon and ZrO2) by the NTA
assisted spreading of molybdenum trioxide with cobalt carbonate, or ammonium heaptamolybdate with
cobalt carbonate was investigated. The selected prepared catalysts were characterized by X-ray
diffraction, N2 physisorption, O2 chemisorption and activity in thiophene (TH) at 1.0 MPa and 400 °C or 1benzothiophene (BT) at 1.6 MPa and 360 °C HDS reaction in the gas phase. It was found that NTA
dissolved the low soluble precursors (MoO3 with CoCO3 or the mixture of ammonium heptamolybdate with
CoCO3) at NTA/(Co+Mo) molar ratio of 0.3-1.0/1.0, which allowed the deposition of the compounds onto
the supports by impregnation. The NTA systematically increased the promotion effect of Co in the sulfided
catalysts in comparison to samples prepared without NTA from ammonium heptamolybdate and cobalt
nitrate. The promotion effect of Co was expressed as ratio of activity of CoMo catalyst and its Mo
counterpart and NTA increased it by the factor 1.13-1.58 for the studied supports.
The research into highly active catalysts for hydrodesulfurization (HDS) reaction is of actual importance
due to increasingly stringent regulations on sulfur level in liquid fuels, processing of crude oil of
progressively deteriorating quality, and increasing demand on the hydrogen management of refineries
(Smith et al., 2012) . The conventional HDS catalysts are CoMo, NiMo or NiW sulfides supported on
gamma-Al2O3 (Topsøe et al., 1996). The catalysts have been recently also studied for hydrotreating of
crude oil alternatives such as bio oils (Baladincz et al., 2012). The preparation of these catalysts is mostly
based on impregnation of the support with aqueous solutions of well soluble salts ammonium
heptamolybdate and cobalt nitrate followed by calcination and sulfidation. New concepts of improving HDS
activity of CoMo sulfide phase are searched among employing alternative supports (Breysse et al., 2003)
or methods of CoMo deposition. For example, we have previously reported on high capacity of activated
carbons to adsorb about 30 wt.% MoO3 from the slurry MoO3/H2O in the form active in HDS reaction and
accessible for activity promotion by Co (Kaluža et al., 2001). Over the zirconium dioxide support, the effect
of employing nitrilotriacetic acid (NTA) for the deposition of ammonium heptamolybdate with cobalt nitrate
or molybdenum trioxide with cobalt carbonate was manifested by the increase in HDS activity by the factor
1.2-1.7 (Kaluža et al., 2012). Similar improvement has been reported for the conventional support Al2O3
(e.g. Hensen et al., 2002). The purpose of the present work was to investigate the effect of NTA on
promotion of hydrodesulfurization activity in CoMo catalyst supported onto gamma-alumina, activated
carbon (C), and zirconium dioxide.
2.1 Supports and reference catalysts
The supports and reference catalysts were crushed and sieved to a particle size fraction of 0.16-0.32 mm.
Carbon support was the commercial active carbon GA-05 (Slovenské lučobné závody, Slovak Republic)
produced from wood. It was refluxed several times with distilled water to remove alkali and dried in a rotary
vacuum evaporator. Alumina support was the commercial product AKZO HDS-000-1.5 (AKZO Chemicals,
2The Netherlands), which is intended for hydrotreating catalysts. It contained 1.3 wt.% of SO4 . The ZrO2
was purchased from Alfa Aesar (product no. 043815, Germany). The following industrial gamma-Al2O3
supported catalysts were used for comparison: Mo(BASF) containing 15.0 wt.% MoO3 (Mo/Al2O3, M8-30,
BASF, Germany) and CoMo(KF756) containing 3.2 wt% CoO and 15.5 wt.% MoO3 (CoMo/Al2O3, KF 756,
Albemarle, the Netherlands).
2.2 Catalysts preparation
Co and Mo were deposited onto the supports to achieve the molar ratio Co/(Co+Mo) equal to 0.3. The Mo
content in carbon and gamma-alumina supported catalysts was chosen to correspond to 13.0 wt.% of
MoO3, which was slightly below the saturated adsorption loadings. The full capacity of ZrO2 to disperse Mo
(saturated adsorption monolayer density 3.5 at. Mo nm ) was used because this support exhibited low
surface area (see Table 1). That capacity corresponds to the loading 8.3 wt. % MoO3. The relation among
support surface area, saturated adsorption loading and HDS activity was discussed in our previous papers
about carbon supported catalysts (Kaluža et al., 2001) and gamma- Al2O3 supported catalysts (Kaluža et
al., 2005). The surface areas of the supports studied are summarized in Table 1.
The catalysts were prepared by two methods: i) conventional consecutive impregnation and ii) the
impregnation with the use of nitrilotriacetic acid (NTA).
i) The support (5 g) was mixed with aqueous solution of ammonium heptamolybdate (20 ml) and it was
shaken for 1 h. It was dried in a rotary vacuum evaporator at 95 °C for 1 h and calcined in air flow
at 400 °C for 1 h with a temperature ramp of 6 °C min . Part of the Mo sample (2.5 g) was impregnated
with the solution of Co(NO3)2 (10 ml), and it was dried and calcined in the same way.
(ii) The support (2.5 g) was immersed into 20 ml of the aqueous solution containing the ammonium
heptamolybdate and NTA, or ammonium heptamolybdate, cobalt nitrate and NTA for 1 h. The sample was
dried in a vacuum evaporator at 95 °C for 1 h and it was not calcined. The Mo samples and CoMo samples
supported on carbon and Al2O3 were prepared with NTA/Mo = 1 and NTA/Co = 1, respectively. The
solution for impregnation of the ZrO2 were prepared from MoO3 and NTA, or MoO3, CoCO3, and NTA with
molar ratio NTA/Mo = 1, or NTA/(Co+Mo) = 1, respectively. The support (2.5 g) was immersed into this
solution and the slurry was mixed for 1 h. The sample was dried in vacuum evaporator at 95 °C for 1 h and
it was not calcined.
2.3 Catalysts characterizations
N2 adsorption isotherms were measured using a Micromeritics ASAP 2010M instrument. Before the
measurements, the samples were evacuated at 110 °C for 12 h. Specific surface area, S(BET), specific
surface area of the mesopores, S(M), and the volume of the micropores, V(Micro), were determined by the
Brunauer–Emmett–Teller (BET) procedure and t-plot method (Table 1). The volume of pores V(Total) was
calculated from the amount of N2 adsorbed at p/p0 = 0.98. All textural parameters were normalized per
gram of the sample.
The X-ray diffraction data were measured using a Philips X’Pert MPD system in Bragg–Brentano reflecting
geometry using Co Ka radiation (40 kV, 30 mA) with wavelength 0.178897 nm and a secondary graphite
monochromator. The data were collected in the range of 10–80 ° 2 theta, at the rate of 0.02 ° per 1.6 s.
2.4 Hydrodesulfurization reactions
The model reactions were HDS of thiophene (TH) at 1.0 MPa and 1-benzothiophene (BT) at 1.6 MPa in
the gas phase in a fixed bed flow reactors. The feed rates of TH, F(TH), and hydrogen, F(H2), were 0.43
mmol h and 1.1 mol h , respectively. The catalyst charge, W, was 0.01 g and it was diluted with an inert
corundum. The catalyst was presulfided in-situ by a H2S/H2 mixture (1:10) at atmospheric pressure with
the following temperature program: ramp 6 °C min to 400 °C and dwell 1 h at 400 °C. The feed TH/H2
was introduced at the temperature of 400 °C and the pressure of 1 MPa. The conversion x(TH) was
determined at 400 °C using a gas chromatograph (Hewlett-Packard, 4890D, Germany); it was defined as
x(TH) = (n0(TH) – n(TH))/n0(TH), where n0 and n are the initial and final number of moles.
The HDS of 1-benzothiophene (BT) was performed at 360 °C. Before the measurements, the catalysts
were sulfided as described above. The composition of the feed was 16 kPa of BT, 200 kPa of decane and
1384 kPa of hydrogen. The catalyst charge, W, was 0.02-0.2 g depending on the catalyst activity and it
was diluted with an inert corundum. The reaction was run at three feed rates of BT, F(BT): 7.7 mmol h ,
10.3 mmol h and 15.5 mmol h . Steady state was reached in 30 min after each change in the feed rate.
The reaction mixture was analyzed on a gas chromatograph (Hewlett-Packard, 6890 series, Germany)
equipped with a capillary column (HP-5, 30 m, 0.53 mm, 1.5 μm). Dihydrobenzothiophene (DH) and
ethylbenzene (EB) were identified in the reaction products. The relative compositions a(BT), a(EB) and
a(DH) and conversions x(BT), x(EB), and x(DH) were defined as a(BT) = (1-x(BT) = n(BT)/n0(BT), a(EB) =
x(EB) = n(EB)/n0 (BT), a(DH) = x(DH) = n(DH)/n0(BT), where n0(BT), n(BT), n(EB), and n(DH) are the
initial and final number of moles.
The empirical pseudo-first-order rate constants of thiophene HDS k(TH) and ethylbenzene formation k(EB)
were calculated from the dependence of the conversion x(TH) and relative composition a(EB) within the
range 0.05-0.95 on space time W/F and it was normalized per unit weight of sulfided catalyst. The relative
activity A(Rel) was expressed as a ratio of the rate constants of the prepared catalysts and the rate
constant of the reference industrial Mo catalyst BASF M8-30 (15 wt.% MoO3, gamma-Al2O3 support). The
promotion effect of Co was defined as a ratio of the activity of CoMo catalyst and its Mo counterpart.
3. Results and discussion
The concept of conventional impregnation form aqueous solutions is based on consecutive deposition of
the metals (Mo first, Co second) because cobalt molybdates precipitate is normally formed by the reaction
of ammonium heptamolybdate and cobalt nitrate. Calcination at temperature above 350 °C is applied to
decompose the Mo salt prior to Co deposition. The presence of NTA, however, prevents the precipitation
reaction by formation of well soluble metal complexes. The impregnation method with the use of NTA was
found to be convenient to deposit the metals onto the supports in one impregnation step. Furthermore, the
chelating power of NTA is so strong that it allowed the dissolution of MoO3 and, surprisingly, also the
dissolution of the mixture of MoO3 and CoCO3 (Kaluža et al., 2012). Another advantage of this method was
that addition of NH4OH was not needed to keep the precursors dissolved. Ammonia forms ammonium
sulfide during in situ sulfidation, which leads to plugging of the reaction apparatus if the reactor exit is not
sufficiently heated. This advantage is particularly important for preparation of activated carbon supported
catalysts because the surplus of ammonia can not be removed from the surface by calcination due to the
support oxidation in air.
The textural and structural parameters of the selected CoMo catalysts were studied by N2 physisorption
and X-ray diffraction. The X-ray diffraction did not detect presence of crystalline phase of NTA, Mo or Co
species in the catalysts after drying or sulfidation. Only the monoclinic phase of ZrO2 (baddeleyite) and low
intensity diffuse peaks of cubic gamma-Al2O3 supports were found in the catalysts. The N2 adsorption
isotherms and textural parameters of the selected samples are shown in Table 1 and Figure 1. It was
Table 1: Textural parameters of the supports, reference catalysts and selected sulfided catalysts
found that the activated carbon and activated carbon supported sample exhibited high volume of
micropores, which was manifested by more than 4 fold higher values V(Micro) and more extensive knee of
the isotherms at low partial pressures (isotherms of type I) in comparison to the samples containing the
oxidic supports (isotherms of type IV). In contrast, total pore volume V(Total) of the carbon and Al2O3
containing samples were similar. The surface areas S(BET) of the carbon containing samples were thus
unrealistically large. To avoid the influence of the microporosity of activated carbon, the mesoporous
surface areas S(M) were calculated by t-plot method. It is seen from Table 1 that deposition of the active
phase with the assistance of NTA and sulfidation of the sample did not decrease the S(M) values of the
original supports. The values remained in the range typical for the HDS catalysts with exception of the
relatively new type of support the monoclinic ZrO2.
The rate constants of thiophene HDS, k(TH), and benzothiophene HDS, k(EB), over the studied catalysts
are summarized in Table 2. The activities of the catalysts normalized to the reference Mo/Al2O3 catalysts
BASF are shown in Figure 2 along with the promotion effect of Co. First, it was found that activated carbon
supported Mo and CoMo catalysts exhibited more than 2-fold activities in comparison to the counterparts
supported on oxidic supports. Secondly the studied catalysts resulted in the same activity ranking in both
model reactions i.e. HDS of thiophene and benzothiophene at 400 and 360 °C, respectively, despite the
fact that HDS of benzothiophene was slightly more sensitive to the NTA use than HDS of thiophene. Third,
the use of NTA during the Co and Mo deposition systematically increased the promotion effect of Co. For
the reaction of thiophene and benzothiophene, the promotion increased by the factor 1.25 and 1.23 for
gamma-Al2O3 supported catalysts, 1.13 and 1.28 for C supported catalysts and 1.25 and 1.58 for ZrO2
supported catalysts, respectively.
The effect of NTA over the studied supports (Table 2, Figure 2) is undoubtedly combination of several
factors. The references to the numerous previous literature explanations can be found in the recent paper
(Lélias et al., 2009). NTA improves the dispersion of metals on the support. Without NTA, the coarsegrained crystalline phase is deposited during drying. In the presence of NTA, gel-like phase is deposited
which transforms to fine-grained solid during sulfidation. Before sulfidation, NTA ligands separate metal
ions from the support and from each other; dissolution of Co in Al2O3 and formation of hard to sulfide
Co3O4 is suppressed. The complexing of Co delays its sulfidation until MoS2 structures are formed and
ready for decoration with Co atoms. NTA promotes the formation of the Type-II Co(Ni)-Mo-S phase
(weaker interaction with support), which is more active than the Type-I Co(Ni)-Mo-S phase (stronger
interaction with support). The present work contributed with the additional activity data (for instance, NTA
effect in TH HDS and have been evaluated only at atmospheric pressure in the literature) and provided
novel view of data and their analysis (activities of conventional and NTA catalysts of the same composition
were compared and the NTA effect on promotion has not been evaluated over Al2O3, C, and ZrO2
Table 2: Catalytic activities k(TH) and k(EB) in thiophene and 1-benzothiophene HDS at 1.0 MPa and 400
°C and 1.6 MPa and 360 °C, respectively
N adsorbed, cm (STP) g
Relative presure (p/p0)
Figure 1: Adsorption isotherms of N2 at -196 °C over the supports and sulfided CoMo catalysts prepared
with the assistance of NTA.
Mo and CoMo prepared without NTA
Mo and CoMo prepared with NTA
Promotion effect A(Rel, CoMo) / A(Rel, Mo)
Benzothiophene HDS, A(Rel)
Thiophene HDS, A(Rel)
Figure 2: Increase in promotion effect of Co by NTA in thiophene and benzothiophene HDS.
The support effect is the main factor governing the activity of Mo and CoMo catalysts. The carbon
supported Mo and CoMo catalysts exhibited more than 2 times higher HDS activities than their Al2O3 and
ZrO2 supported counterparts. The employing of the chelating agent nitrilotriacetic acid in the preparation of
the CoMo catalysts supported on gamma-Al2O3, activated carbon, and monoclinic-ZrO2 systematically
increased the promotion effect of Co in hydrodesulfurization reaction of thiophene and benzothiophene at
high pressure by the factor 1.13-1.58.
Authors gratefully acknowledge the Albemarle Company (The Netherlands) and the BASF Company
(Germany) for providing reference catalysts and the Czech Science Foundation (grant numbers
P106/11/0902 and 104/09/0751) for the financial support.
Baladincz P., Tóth C., Hancsók J., Production of diesel fuel via hydrogenation of rancid lard and gas oil
mixtures, Chemical Engineering Transactions 29, 1237-1242.
Breysse M., Afanasiev P., Geantet C., Vrinat M., 2003, Overview of support effects in hydrotreating
catalysts, Catal. Today 86, 5-16.
Hensen E.J.M., de Beer V.H.J., van Veen J.A.R., van Santen R.A., 2002, A refinement on the notion of
type I and II (Co)MoS phases in hydrotreating catalysts, Catal. Lett. 84, 59-67.
Kaluža L., Gulková D., Vít Z., Zdražil M., 2012, CoMo/ZrO2 Hydrodesulfurization catalysts prepared by
chelating agent assisted spreading, Catal. Lett. 142, 969–974.
Kaluža L., Vít Z., Zdražil M., 2005, Preparation and properties of filled monolayer of MoO3 deposited on
Al2O3 supports by solvent-assisted spreading, Appl. Catal. A: General 282, 247-253.
Kaluža L., Zdražil M., 2001, Carbon-supported Mo catalysts prepared by a new impregnation method
using a MoO3/water slurry: Saturated loading, hydrodesulfurization activity and promotion by Co,
Carbon 39, 2023-2034.
Lélias M.A., Kooyman P.J., Mariey L., Oliviero L., Travert A., van Gestel J., van Veen J.A.R., Maugé F.,
2009, Effect of NTA addition on the structure and activity of the active phase of cobalt-molybdenum
sulfide hydrotreating catalysts, J. Catal. 267, 14-23.
Smith R., Zhang N., Zhao J., 2012, Hydrogen integration in petroleum refining, Chemical Engineering
Transactions 29, 1099-1104.
Topsøe H., Clausen B.S., Massoth F.E., 1996, Hydrotreating Catalysis. Springer, Berlin, Germany.